Dottorato di ricerca in Fisica XXVII Ciclo
Ab initio modelling of positive muon implantation sites in crystalline solids
Chiar.mo Prof. Cristiano Viappiani
Chiar.mo Prof. Roberto De Renzi
Dottorando: Pietro Bonfà
List of Papers ix
1. Introduction and motivation 3
1.1. Outline of the thesis . . . 5
2. A short introduction to µSR 7 2.1. Brief history . . . 8
2.2. Muon production . . . 9
2.3. Implantation and decay . . . 11
2.4. The µSR observable: the asymmetry . . . . 12
2.4.1. Continuous and pulsed puon beams . . . 16
2.4.2. Experimental setup . . . 17
2.5. Probing magnetic order . . . 19
2.5.1. Contributions to the local field at the muon site 19 2.5.2. Static and dynamic local fields . . . 22
2.6. Quantum description of the dipolar interaction . . . . 25
2.7. Identification of muon sites . . . 28
2.7.1. Experimental approaches . . . 28
2.7.2. Theoretical approaches . . . 29
3. A short introduction to DFT 31 3.1. The Hohenberg-Kohn theorems . . . 32
3.1.1. One to one mapping . . . 32
3.1.2. Variational principle . . . 33
3.1.3. V-representability and N-representability . . . 34
3.1.4. Kohn Sham iterative scheme . . . 35
3.1.5. Exchange and correlation approximations . . . 40
3.1.6. Reciprocal space sampling . . . 41
3.2. Ionic contribution to the total energy . . . 43
3.3. Basis sets . . . 44
3.3.1. Plane Waves . . . 45
3.3.2. Linearized Augmented Plane waves . . . 49
3.4. DFT for muon site identification . . . 51
3.4.1. Alloys, impurities and defects . . . 51
3.4.2. The muon as a charged impurity . . . 53
3.4.3. Double Adiabatic Approximation . . . 57
4. Iron Pnictides: studying the unperturbed system 59 4.1. Introduction . . . 60
4.2. LaFeAsO . . . 61
4.3. FeTe . . . 64
4.4. LaCoPO . . . 66
4.5. Discussion . . . 73
5. Fluorides: a more rigorous method 75 5.1. The supercell approach . . . 77
5.2. LiF . . . 78
5.3. YF3 . . . 81
5.4. Discussion . . . 84
6. MnSi and Cu: from classical to quantum 87 6.1. MnSi . . . 87
6.2. Copper . . . 92
6.3. Discussion . . . 97
7. T0-La2CuO4: field glasses for µSR 99 7.1. Introduction . . . 100
7.2. Electrostatic potential . . . 101
7.3. Muon site estimation . . . 103
7.4. Ground state energy . . . 105
7.5. Discussion . . . 106
8. Conclusions 109 A. Technical details of the simulations 113
A.1. LaFeAsO . . . 113
A.2. FeTe . . . 113
A.3. LaCoPO . . . 114
A.4. LiF and YF3 . . . 115
A.5. MnSi . . . 116
A.6. Cu . . . 117
A.7. T0-La2CuO4 . . . 117
B. The DBO code 121 C. Solving the Schrödinger equation 125 D. Codes 129 D.1. DBO . . . 129
D.2. Unfold . . . 129
In this thesis, a computationally efficient method for identifying in- terstitial muon sites in crystalline solids is presented. An accurate determination of muon embedding positions and effects is important for muon spin rotation and relaxation experiments since it can signif- icantly widen the capabilities of this experimental technique. Indeed, these information are usually unknown to the experimenter and in most cases it is not possible to characterize the muon sites and the muon induced perturbation from experimental knowledge.
The approach proposed in this thesis is based on ab initio Density Functional Theory (DFT) simulations and it was designed to provide a companion tool to assist muon spin rotation data analysis. The first principles determined muon stopping site(s) and the expected perturbation produced by the muon implantation have been compared to muon spin rotation and relaxation results in a series of textbook cases that have been extensively characterized experimentally.
It is also highlighted that the estimation of the ground state energy of the muon (also referred to as zero point motion energy) is cru- cial in order to distinguish between trapping and non-trapping muon sites. In order to keep the computational load of the ab initio sim- ulations within the bounds of standard computer clusters capacities, we approximate the total Hamiltonian of the system introducing a Born-Oppenheimer separation between the degrees of freedom of the muon and those of the nuclei and of the electrons. This approach has been referred to as double adiabatic approximation in literature. The method is found to be sufficiently accurate as well as computation- ally feasible when an algorithmic procedure to efficiently perform the simulations is introduced.
The successful results obtained so far include the identification of muon sites in iron pnictide superconductors, the study of F-µ-F cen-
tres in fluorides, muon diffusion in Copper and the recent identifica- tion of muon sites in MnSi and T0-La2CuO4. All these cases confirm the validity of the DFT approach and emphasize the importance of accurate muon site predictions.
My sincere gratitude goes to my advisor, Prof. Roberto De Renzi. His quick and enlightening physical intuition provided the fundamental guidance for all the work hereby presented. However, it would be unfair to avoid mentioning how the inspiring discussions, the effective ideas, his humor and positive attitude in general made working in Parma amazing. In brief, having Roberto De Renzi as advisor has been an honour and a pleasure.
I am also grateful to Dr. Fabio Bernardini for his fundamental scientific contribution to this work, for the constant and considerable support and for his precious training in density functional theory.
The same holds true for Dr. Gianni Profeta, who introduced me the fundamental concepts behind computational physics.
Special thanks are also due to Dr. Giuseppe Allodi for his constant and essential support during NMR sessions.
It has also been a pleasure to continue the collaboration with the advisor and the co-advisor of my master degree theses, Prof. Pietro Carretta and Dr. Samuele Sanna. At the same time I learned a lot from the collaboration with Dr. Gianrico Lamura, Dr. Toni Shiroka, Dr. Giacomo Prando and Dr. Franziska Hammerath, Dr. Marcello Mazzani.
Part of the work discussed in this thesis arises from the discussion and the excellent work of a number of collaborators that I will not list here because, for sure, I would forget someone. To mention but a few, it has been a pleasure to meet and discuss with doctors Gwendolyne Pascua, Johannes Möller, Franz Lang, Hubertus Luetkens, Alex Am- ato and Rustem Khasanov.
Finally, I cannot refrain from expressing my grateful acknowledge- ments to the ping pong people, to Michela for her unbelievable pa- tience and to my parents for being my parents!
List of papers
The papers published during the Ph.D. are divided in two sections.
This thesis is based on the work collected in articles from section A which deal partially or entirely with the identification of muon sites.
Other results concerning superconducting and magnetic materials are reported in papers listed in section B. Pre-prints and submitted papers are listed in section C.
1. “Ab initio strategy for muon site assignment in wide band gap fluorides”.
F. Bernardini, P. Bonfà, M. Massidda, R. De Renzi Physical Review B
2. “A magnetic glassy phase in Fe1+ySexTe1−x single crys- tals”.
G. Lamura, T. Shiroka, P. Bonfà, S. Sanna, F. Bernardini, R.
De Renzi, R. Viennois, E. Giannini, A. Piriou, N. Emery, M.R.
Cimberle, M. Putti
Journal of Physics-Condensed Matter DOI:10.1088/0953-8984/25/15/156004
3. “Common effect of chemical and external pressures on the magnetic properties of RCoPO (R = La, Pr)”.
G. Prando, P. Bonfà, G. Profeta, R. Khasanov, F. Bernardini, M. Mazzani, E.M. Bruning, A. Pal, V.P.S. Awana, H.J. Grafe, B. Buchner, R. De Renzi, P. Carretta, S. Sanna
Physical Review B
4. Understanding the µSR spectra of MnSi without mag- netic polarons
A Amato, P Dalmas de Réotier, D Andreica, A Yaouanc, A Suter, G Lapertot, IM Pop, E Morenzoni, P Bonfà, F Bernar- dini, R De Renzi
Physical Review B
5. “Effect of external pressure on the magnetic properties of LnFeAsO (Ln = La, Ce, Pr, Sm)”.
R. De Renzi, P. Bonfà, G. Prando, P. Carretta, R. Khasanov, A. Amato, H. Luetkens, M. Bendele, F. Bernardini, S. Massidda, A. Palenzona, M. Tropeano and M. Vignolo
Superconductor Science and Technology DOI:10.1088/0953-2048/25/8/084009
6. “Playing quantum hide-and-seek with the muon: local- izing muon stopping sites”.
J. S. Möller, P. Bonfà, D. Ceresoli, F. Bernardini, S. J. Blun- dell, T. Lancaster, R. De Renzi, N. Marzari, I. Watanabe, S.
Sulaiman, M. I. Mohamed-Ibrahim Physica Scripta
DOI:10.1088/0031-8949/88/06/068510 Section B
7. Poisoning effect of Mn in LaFe1−xMnxAsO0.89F0.11: Un- veiling a quantum critical point in the phase diagram of iron-based superconductors F Hammerath, P Bonfa, S Sanna, G Prando, R De Renzi, Y Kobayashi, M Sato, P Car- retta Physical Review B DOI:10.1103/PhysRevB.89.134503 8. Tuning the magnetic and structural phase transitions of
PrFeAsO via Fe/Ru spin dilution
Yuen Yiu, Pietro Bonfà, Samuele Sanna, Roberto De Renzi, Pietro Carretta, Michael A. McGuire, Ashfia Huq, and Stephen E. Nagler
Physical Review B DOI:10.1103/PhysRevB.90.064515
nium for iron substitution in LaFe1−xRuxAsO Marcello Mazzani, Pietro Bonfà, Giuseppe Allodi, Samuele Sanna, Al- berto Martinelli, Andrea Palenzona, Pietro Manfrinetti, Marina Putti, Roberto De Renzi
physica status solidi (b) DOI:10.1002/pssb.201350237
10. “s-wave pairing in the optimally-doped LaO0.5F0.5BiS2 superconductor”.
G. Lamura, T. Shiroka, P. Bonfà, S. Sanna, R. De Renzi, C.
Baines, H. Luetkens, J. Kajitani, Y. Mizuguchi, O. Miura, K.
Deguchi, S. Demura, Y. Takano, and M. Putti
Physical Review B (R) DOI:10.1103/PhysRevB.88.180509 11. “Role of in-plane and out-of-plane dilution in CeFeAsO:
Charge doping versus disorder”.
G. Prando, O. Vakaliuk, S. Sanna, G. Lamura, T. Shiroka, P.
Bonfà, P. Carretta, R. De Renzi, H.-H. Klauss, C. G. F. Blum, S. Wurmehl, C. Hess, and B. Büchner
Physical Review B
12. “Onset of magnetism in optimally electron-doped LFe1−xRuxAsO1−yFy (L = La, Nd, or Sm) superconductors around x =1 /4”.
S. Sanna, P. Carretta, R. De Renzi, G. Prando, P. Bonfa, M.
Mazzani, G. Lamura, T. Shiroka, Y. Kobayashi, M. Sato, R. De Renzi
Physical Review B
13. Crossover between magnetism and superconductivity in LaFeAsO with low H-doping level
G Lamura, T Shiroka, P Bonfà, S Sanna, R De Renzi, F Caglieris, MR Cimberle, S Iimura, H Hosono, M Putti
Journal of Physics: Condensed Matter DOI:10.1088/0953-8984/26/29/295701 Section C
14. Efficient and reliable strategy for identifying muon sites based on the Double Adiabatic Approximation
P Bonfà, R De Renzi
submitted to: The Journal of Chemical Physics C
15. DFT assisted muon embedding site assignment: the case of T0-La2CuO4 P. Bonfà, F. Bernardini, R. De Renzi, G. Pascua, H. Luetkens
Comments on my participation In paper 1) I have carried out the developments, all the calculations and I have written the manuscripts.
In papers 2), 3) and 4) I have carried out the DFT simulations and written part of the manuscript. In paper 5) I have taken part to the analysis of the muon site. In paper 6) I have done part of the DFT simulations and written part of the manuscript. Paper 7) is the sum of NMR and µSR measurements. I analysed an discussed the µSR part.
Paper 8) is the sum of neutron scattering and µSR measurements.
I analysed an discussed the µSR part. In paper 9) I have done the DFT simulations and I took part to the NMR measurements and simulations and I wrote part of the manuscript. In papers from 10) to 13) I took part to the measurements. In manuscripts 14) and 15) I have done/developed all the DFT simulations as well as written the manuscripts.
µSR Muon Spin rotation and Relaxation spectroscopy. 3–5, 7, 99, 106, 111
AFM antiferromagnetic. 22, 63, 65, 101, 111 APW Augmented Plane Waves. 49, 50 BO Born Oppenheimer. 36, 43, 44, 56, 98
DAA Double Adiabatic Approximation. 57, 77, 86, 87, 89, 90, 92, 97, 105, 110, 111, 118, 121, 129
DBO Double Born Oppenheimer. 58, 90, 91, 94–96, 117, 129
DFT Density Functional Theory. 4, 5, 29–32, 34, 38, 40, 45, 51, 53, 55, 60, 61, 68, 69, 75, 78–87, 89, 99, 101, 104, 106, 109–111, 113, 117, 118
DMFT Dynamical Mean Field Theory. 101, 118 FM Ferromagnetic. 66, 68, 71, 116
FP Full Potential. 49, 60, 61, 101, 113–116
GGA Generalized Gradient Approximation. 41, 101, 113, 116, 118, 119
GSE Ground State Energy. 54, 56, 57, 63, 65, 72, 77–79, 81, 85, 87, 97, 105, 110
HF Hartree Fock. 4, 29
Acronyms HK Hohenberg and Kohn. 32–35
IPSC Iron Pnictides Superconductor. 60, 61, 64, 73–75, 89, 109 KKR Korringa-Kohn-Rostocker. 51, 52
KS Kohn and Sham. 32, 35, 37, 39, 40, 43–45, 47, 58
LAPW Linearized Augmented Plane Waves. 44, 49, 50, 113, 114, 116 LDA Local Density Approximation. 40, 41, 113
MP Monkhorst and Pack. 42, 94, 114, 116–118 NEB Nudged Elastic Band. 94, 97, 117
NMR Nuclear Magnetic Resonance. 3, 4, 8, 18, 63, 99, 101, 102, 106, 107
PAW Projector Augmented Wave. 48, 77, 114
PBC Periodic Boundary Conditions. 29, 52, 55, 91, 96 PBE Perdew Burke Ernzerhof. 114, 116–118
PW Plane Wave. 44, 45, 68, 114, 115, 118
TDDFT Time-Dependent Density Functional Theory. 32
1 Introduction and motivation
The scope behind the study presented in this thesis is the develop- ment of a computational companion tool to assist Muon Spin rotation and Relaxation spectroscopy (µSR) data analysis in a time effective and affordable manner. An efficient, reliable and sufficiently accurate way to study the interstitial sites and perturbations introduced by the positively charged muon in its local neighbourhood in crystalline solids would empower µSR with unprecedented quantitative estima- tion possibilities.
µSR is a powerful experimental technique for all the problems in condensed matter physics which can take advantage of a microscopic magnetometer embedded within the sample, i.e. the muon. Among the many, magnetism and superconductivity are probably the most common, followed by the study of hydrogen-like impurities in semi- conductors, their diffusion and reaction kinetics, and studies of quan- tum diffusion mechanisms [1–3]. µSR is often compared to Nuclear Magnetic Resonance (NMR) in providing information on static and dynamic magnetic fields on a local scale, but, unlike NMR, it can eas- ily be performed in zero applied field (since muons can be produced in fully polarised beams), it is applicable to almost any material and removes the requirement for a radio-frequency to activate the probe.
The price to pay is a large uncertainty in the muon position inside the sample. In parallel and as a part of the development of the experimen- tal technique, a lot of work has been devoted to the determination of muon sites in crystals. A precise characterisation of the muon intersti- tial sites was indeed possible from accurate experimental studies of the
Knight shift, of the level crossing resonance (LCR) and by inspecting asymmetry relaxation rates as a function of applied fields in selected compounds (see for example [4–8]). However, in a large number of cases the muon position and its effect on the hosting system cannot be inferred solely by experimental knowledge and a reliable method to obtain the muon site in condensed matter would be of great value. To this aim, we have selected ab initio methods, and especially Density Functional Theory (DFT) based quantum chemistry approaches, as the computational scheme to perform muon site identification simu- lations and support µSR data analysis.
DFT is a widely accepted framework to solve the Schrödinger equa- tion for an interacting many-body system. Its enormous success is testified by the large set of scientific fields which benefit from the prediction power offered by the computational approaches based on Kohn Sham’s auxiliary system method. Developments in electronic structure methods combined with a continuously increasing comput- ing power can deliver unprecedented accuracies in computational ex- periments on a quantum mechanical perspective. As of today, many experimental techniques rely on DFT to support the data analysis.
In the field of condensed matter, DFT can be used to interpret and predict spectroscopic properties like core-level electron energy loss (EELS) spectra, vibrational infra-red and Raman spectra, NMR and electron paramagnetic resonance spectra (EPR), linear and nonlinear optical spectra [9, 10]. This vast collection of successful results pro- moted DFT simulations as the computational scheme of election for the practical realisation of a tool for µSR data interpretation support.
Identifying muon sites with ab initio approaches is not a new idea.
A lot of attention has been devoted, in the last three decades, to the analysis of muon interactions in solids by means of Hartree Fock (HF), DFT and other simulation techniques (see for example Ref. [11–15]).
The contributions to the development of the experimental technique obtained with computational methods are hardly enumerable. How- ever, in most cases the attention has been mainly devoted to µSR experiments where the interpretation of the experimental data was
1.1. Outline of the thesis elusive or ambiguous. Here we started from the opposite perspective.
In this thesis we choose a set of materials where the muon site is known from the experiment or can be easily checked. On this solid grounds we test the accuracy of a DFT based approach to identify muon sites.
Accomplishing this ambitious task is of course well beyond the abil- ity of any single researcher or group possibilities. However, the re- sults discussed in this thesis and in literature (among the many, see Ref. [16–25]) are promising and call for further investigations.
1.1. Outline of the thesis
In chapter 2 and 3 we introduce the µSR technique and illustrate the basic concepts behind DFT. In chapter 4 we discuss a simple ap- proach to identify muon sites, namely the inspection of the minima of the electrostatic potential of the unperturbed material. This approach is found to be sufficiently accurate for some special cases. However, in general, this crude approximation does not provide satisfying re- sults. Therefore, a better estimation, which takes into account the perturbation introduced by the µ embedding, is discussed in chapter 5. In chapter 6 we improve our method by proposing a simple and yet sufficiently accurate approach to evaluate the ground state energy of the muon, whose effect is found to have relevant consequences on the interstitial site determination task. In chapter 7 we discuss how all the above results are used to unveil the magnetic properties of a material of high scientific interest, namely the T0 structure of La2CuO4. In- deed, the knowledge of the muon site, which in this case happens to be in a low symmetry interstitial position, allows to distinguish among the possible long-range magnetic orders and therefore to determine the ground state magnetic structure. In chapter 8 we conclude the thesis and discuss some perspectives for future developments.
2 introduction to A short µSR
2.1. Brief history . . . . 8 2.2. Muon production . . . . 9 2.3. Implantation and decay . . . . 11 2.4. The µSR observable: the asymmetry . . . . 12 2.4.1. Continuous and pulsed puon beams . . . . 16 2.4.2. Experimental setup . . . . 17 2.5. Probing magnetic order . . . . 19
2.5.1. Contributions to the local field at the muon site . . . . 19 2.5.2. Static and dynamic local fields . . . . 22 2.6. Quantum description of the dipolar inter-
action . . . . 25 2.7. Identification of muon sites . . . . 28 2.7.1. Experimental approaches . . . . 28 2.7.2. Theoretical approaches . . . . 29
µSR is a spectroscopic technique in which implanted positive muons are used as a nanoscopic magnetometer placed within the sample.
This is made possible by two favourable conditions offered by nature:
parity violation in the weak decay and the production of spin polarised µ+beams through the decay of the pion. The experimenter is provided
Figure 2.1.: Header of the first µSR newsletter.
with the time evolution of the direction of the muon spin which can be extracted from the collection of each decay positron as a function of the individual muon lifetime spent within the sample.
The name stands, in the words of the first µSR Newsletter (Fig. 2.1), for “Muon Spin Relaxation, Rotation, Resonance, Research, or what have you” intentionally suggesting the analogy with NMR in which nuclei are used for the same scope.
µSR is often utilised to investigate the magnetic and the supercon- ducting properties of a sample, but it finds wide application also in studies of the effect hydrogen-like impurities in semiconductors, quan- tum diffusion, reaction kinetics and several other fields [2, 26].
In this section, a brief introduction to µSR is presented. For a more detailed description of this technique as well as of the various applications in many field of research, the reader is referred to the several books and review articles [1, 3, 27–29].
2.1. Brief history
The muons arising from the secondary radiation of cosmic rays were first observed in 1936 by C. D. Anderson and S. Neddermeyer. How- ever, the breakthrough that allowed the progress toward the modern µSR technique was the discovery of parity violation in weak decay
2.2. Muon production observed experimentally in 60Co beta decay by Wu et al in 1957 and predicted by Nobel awarded scientists Lee and Yang .
The first proton accelerators offering the intense pion (and hence muon) beams which are needed to perform µSR experiments were first produced at the CERN synchrotron, at JINR in Dubna, at SREL in Berkeley and at Nevis Columbia at the end of the 1950s. Starting from the 1970s, new high-intensity intermediate-energy accelerators were built at laboratories in the Schweizerisches Institut für Nuklearphysik (CH), Los Alamos (USA) and TRIUMF Vancouver (Canada). These new accelerators offered continuous beams (vide infra) two orders of magnitude more intense than the previous accelerators. Shortly after, pulsed muon facilities were realised in ISIS at the Rutherford Appleton Laboratory in UK and KEK in Tsukuba, Japan (now replaced by J- PARC in Tokai) and the new continuous beam facility PSI was built in Villigen (CH).
2.2. Muon production
High intensity collimated muon beams are produced using accelerated protons in a two step process. The collision of two protons or a proton and a neutron initially produces a pion according to
p + p → π++ p + n , (2.1)
p + n → π++ n + n (2.2)
p + n → π−+ p + p (2.3)
The first particle in Eq. 2.1, 2.2 and 2.3 comes from the accelerated proton beam while the second is at rest in a muon production target (usually graphite). The kinetic energy T = c2(m − m0) = m0(γ − 1) of the accelerated proton having quadrimomentum ¯P1i for producing a pion at rest in the muon production target where the neutron with quadrimomentum ¯P2i resides is
P¯1i+ ¯P2i= ¯Pf
2m2p+ 2m2pγ = (2mp+ mπ)2
where we have assumed mn= mp (the intended meaning of the sym- bols should be clear from context). This gives γ = 1 + 2mmπ
p and a threshold kinetic energy of about (γ−1)mpc2= 2mπc2 ∼ 280 MeV. However, for sake of efficiency in the pion production, usu- ally proton beams with energies between 500 and 800 MeV are used.
Pion half life time is just 26 ns and from its decay a positive or negative muon is produced via the two-body decay:
π+→ µ++ νµ (2.4)
π−→ µ−+ ¯νµ (2.5)
It’s worth noting that the negative pion (process in Eq. 2.3) stopping in the production target almost always undergoes nuclear capture be- fore it has a chance to decay. Negative muons may be produced from the in-flight negative pion’s decays (see following) but, as for negative pions, the lifetime of negative muons in matter is reduced by nu- clear capture. For this reason, and also because surviving µ−fall into atomic orbitals extremely close to atomic nuclei, µ+SR is more com- monly used to investigate condensed matter and will be considered in the following.
In the process in Eq. 2.4, since the neutrino has negative helicity and the pion is a spin-less particle, the conservation of momentum implies that muon spin is aligned antiparallel to its momentum in the pion’s rest frame. As a consequence, polarised muon beams are produced in two distinct pion momentum regimes
• selecting muon that arise from π+ at rest near the surface of the muon production target. This method produces a 100% po- larised muon beam with kinetic energies of about 4.1 MeV and a maximum momentum of 29.8 MeV/c. This is the so called
2.3. Implantation and decay
50 MeV ∼ 200 eV
scattering with valence electrons
Epithermal scatter- ing of muonium with atoms and molecules, vacancy formation
”molecules in crystals”
containing µ+ µ+beam
scattering with core electrons
∼ 20 eV
Figure 2.2.: Flow chart showing the processes involved in the slowing down of high-energetic muons in matter.
“surface” or “Arizona” beam. The low momentum character- ising these beams is suited for studying thin samples and tiny single crystals of about 1 mm2.
• By collecting muons from in-flight pion’s decays in a long su- perconducting solenoid. Typical muon beams with a polarisa- tion < 100% and energies of ∼40-50 MeV are produced after momentum selection by bending magnets. As a consequence, muons have appreciably longer stopping ranges in matter and this can be used to overcome thick cryostat walls or pressure cells, thus allowing the exploration of extreme temperature or pressure conditions.
2.3. Implantation and decay
As already discussed, µ+ are directed at the sample as a fully po- larised beam. They slow down loosing energy primarily by ionisation, vacancy formation and bremsstrahlung emission . During the de- celeration, the muon may form a bound state, called muonium, with an electron. The bound state can dissociate during the deceleration and the formation and dissociation process may take place repeatedly.
The muon eventually reaches an interstitial position where it may re- side with the collected electron or (partially) lose it as a consequence of chemical interactions with the electrons of the hosting material.
In several cases muons end up in multiple final states, with different probabilities.
A sketch of the processes involved in the deceleration is shown in Fig. 2.2. Muonium interacts with the host by collisions with the atoms
and radiation damage is produced during the deceleration. However, when muon’s energy eventually drop below the threshold for vacancy production, it still travels ahead for ∼ 100−600 Å . For this reason, the muon usually probes a region of the sample which is far from the initial part of the deceleration path which suffered from radiation damage.
The interactions between the muon and the sample during the de- celeration process most often preserve the muon’s polarisation .
The deceleration time depends on the density of the material and ranges from 100 ps in condensed matter to 10 ns in gases. This time interval is too short to allow a significant loss of polarisation coherence during the early stages of the thermalization in non-magnetic metallic samples where muonium formation is rare. The situation is different in insulators and molecular materials. In this case a discrepancy be- tween the initial muon beam polarisation and the polarisation at the earliest measurable time is not uncommon. This is possibly due to the formation of a muonium precursor that may give rise to a prompt depolarisation usually referred as “missing fraction”. It’s important to mention that, in high field experiments, the initial polarisation of the muons can be slightly different from that of the muon beam, but, in this case, the coherence between the initial polarisation of all incoming muons is preserved.
2.4. The µSR observable: the asymmetry
The average lifetime of the muon is τµ= 2.2 µs and the decay proba- bility follows the well known exponential law e−t/τµ. The weak decay of the muon is a three body process
µ+ → e++ νe+ ¯νµ (2.6) where e+ is a positron and νe and ¯νµ are neutrinos. Parity violation in the weak decay and the conservation of angular momentum imply an asymmetry in the positron emission direction. This is the result on which the entire µSR technique is based. In the weak decay the positron emission probability as a function of its energy is given by
2.4. The µSR observable: the asymmetry
0 0.2 0.4 0.6 0.8 1
0 0.5 1
1 1.5 1
Figure 2.3.: In (a), the probability of emitted positron energy and the relative asymmetry function a are shown (see Eq. 2.4).
In (b), the angular distribution of the positron emission probability for various positron energies is depicted.
dP (∗, θ) d∗dΩ = 1
2πp(∗) (1 + a(∗) cos θ) (2.7) where ∗ = /max (max = 52.8MeV), θ is the angle between muon’s spin and positron emission direction and p(∗) and a(∗) are the rela- tive emission number and the asymmetry functions, given by:
a(∗) = 2∗− 1 3 − 2∗
p(∗) = (∗)2(3 − 2∗) .
Both functions are plotted in Fig. 2.8. Averaging over all positron energies gives
A = ha(˜ ∗)i = Z 1
a(∗)p(∗) d∗ = 1
Substituting ˜A from Eq. 2.8 into Eq. 2.7 and integrating over all positron emission energies one finds that the positrons are emitted predominantly in the direction of the muon spin. Thus, collecting the
µ+ B detector F detector
Figure 2.4.: A simple diagram of the detector’s geometry in a typical µSR experimental setup. Black and orange arrows indi- cate particles’ spin and momentum direction, respectively.
The detectors are identified by capital characters U, L, F, B respectively for upper, lower, forward and backward.
positron counts in a detector at a given direction as a function of time, it is possible to follow the muon spin dynamics.
When immersed in a magnetic field B forming an angle with the initial muon polarisation sµ(t0) the muon will precess around it with an angular frequency ωµ given by
ωµ= γµ|B| (2.9)
where γµ= 2me
µgµ is the gyromagnetic ratio of the muon. The exper- imental values  gµ= −2.0023318418(13), mµ= 1.883531475(96) × 10−28kg give γµ/2π= −135.538817(7) MHz/T.
The time dependent count of detected positrons can be written as:
Ne(i)+(t) = N0(i)ne−t/τµh1 + ˜AP(i)(t)i+ B0(i)o (2.10) where i is a label enumerating the detectors and, with reference to the scheme shown in Fig. 2.4, ranges from 1 to 4 and refers to the Upper, Lower, Backward and Forward detectors, B0 is a time-independent background of uncorrelated counts and N0 is a normalizing rate con- stant. The decreasing exponential accounts for the decay of the µ+
2.4. The µSR observable: the asymmetry
0 1 2 3 4 5 6
Figure 2.5.: Schematic illustration of a µSR acquisition histogram.
The figure shows the exponential decay of the muons (dot- ted line) as collected by an appropriate couple of opposite detectors in the presence of a local magnetic field form- ing an angle with the initial muon spin (for example the forward and backward scintillators reported as NF and NB in the figure). The signal will overshoot or stay un- der the standard exponential decay during the µ+lifetime reflecting the time dependence of the muon polarization.
and P(i)(t) is the time evolution of the muon polarisation in the di- rection of the i-th detector.
If the muons stop in equivalent sites within the lattice and experi- ence a unique perpendicular magnetic field (either internal or applied) with respect to the detector i and the initial beam polarization, the spins precess around the field and the emission in the i direction is given by inserting
P(i)(t) = cos(ωµt + θ(i)) (2.11) in Eq. 2.10, where θ(i) is the initial phase of the muon relative to the i-th detector. The signal coming from opposite detectors shows the typical decay plus oscillation sketched in Fig. 2.5.
It’s possible to remove the dependence from the exponential decay
by introducing the asymmetry function:
A(t) = N(i)(t) − N(j)(t)
N(i)(t) + N(j)(t) (2.12) where i and j are couples of opposite detectors, for example backward and forward or upper and lower. Substituting Eq. 2.11 and Eq. 2.10 into Eq. 2.12 and disregarding the constant background one gets
(α − 1) + ˜AαP(i)− P(j)
(α + 1) + ˜A αP(i)+ P(j) (2.13) where α = N0(i)/N0(j). This last parameter takes into account the differences in finite detectors’ geometry, efficiency between i and j de- tectors and not perfect initial beam polarisation. In general α takes values close to 1. Once the differences among the detectors that in- fluence the asymmetry have been corrected using
A∗(t) = αN(i)(t) − N(j)(t)
αN(i)(t) + N(j)(t) (2.14) by substituting Eq. 2.11 into Eq. 2.14 one gets
max(A∗(t)) = ˜A . (2.15) Practically, max(A∗(t)) ' 0.25 due to lower relative efficiency in the detection of high energy large asymmetry positrons and to the finite size of the detector array.
2.4.1. Continuous and pulsed puon beams
Muon spectroscopy facilities offer two kind of muon beams: continuous and pulsed. These two approaches offer complementary potentialities.
In continuous-µSR, muons arrive nearly continuously and are detected by muon’s detector one by one (see Fig. 2.4). Each muon hitting the muon detector starts the electronic clock and the system awaits for the decay event to be detected in one of the positron detectors. It may happen anyway that two muons reach the sample before a decay event
2.4. The µSR observable: the asymmetry is detected. This prevents the association of the decayed positron to its parent muon. This fact constitutes the main source of background noise in continuous-µSR and limits the maximum incident muon rate.
On the other hand, one of the main advantages of the continuous beam facilities is the excellent time resolution, which can be of a few tenths of ps.
In pulsed-µSR a bunched beam of muons (up to more than 103 muons per pulse, at ISIS) reaches the sample and the zero time ref- erence is synchronised with the beam pulses’ extraction. Two con- straints apply to the time structure of the pulsed beam: the time length of the pulses must be considerably shorter than the muon life- time, while the repetition time must be much longer than the muon lifetime. The first condition constitutes the main disadvantage of this kind of facilities. The time resolution of the µSR signal is limited by the muon pulse width and, for example, a band width of about 10 MHz (pulse width of 70 ns) will result in a maximum detectable local field of about 600 G. The pulsed muon technique has the advantage of using all muons entering the sample (contrary to continuous µSR where many muons are discarded due to multiple decay events in a single acquisition time window) and provides a signal almost free from background counts. Asymmetry measurements up to 10τµ are possi- ble due to both the negligible background and the possibility of using a higher rate of incoming muons with respect to continuous beams.
2.4.2. Experimental setup
For sake of simplicity, in the next section we will introduce the typical experimental setup of a continuous beam facility.
The muon coming from the beam-line and its decay positron are usually detected by fast plastic scintillation and fast phototube de- tectors (Fig. 2.4). The muon detector is thin enough to let the muon pass through and allows to set the t = 0 reference. After its detection an electronic timer is started and the time between implantation and the positron emission is recorded. The positrons are detected by an array of detectors and µSR data are acquired as a set of time-series histograms.
Three experimental configurations are possible depending on the
µ+ B detector F detector
Figure 2.6.: LF-µSR experimental setup. Red lines represent external field flux lines. Black and orange arrows indicate particles’
spin and momentum direction, respectively.
direction of the applied field relative to the initial muon spin polari- sation:
Zero-field configuration (ZF-µSR) This experimental setup is char- acterised by the absence of external magnetic fields. Due to the ex- treme sensitivity of the µSR technique, usually cancellation of the Earth’s magnetic field is also required. This approach is particularly useful in materials with spontaneous magnetic properties since µSR can be used to probe samples without the application of an external field thus providing complementary information with respect to NMR.
In magnetic materials, this method offers a measure of the evolution of the order parameter as a function of temperature or pressure since the precession frequency is proportional to the magnetisation (or the staggered magnetisation) of the system.
Longitudinal-field configuration (LF-µSR) In this experimental con- figuration the magnetic field HL is applied along the direction of the initial muon polarisation (Fig. 2.6). Longitudinal fields are generally used in combination with zero-field experiments to disclose the nature of the internal magnetic field distribution, the presence of dynamic processes (see Refs. [1, 27] for details) or in Level Crossing Resonance (LCR) experiments.
2.5. Probing magnetic order
µ+ B detector F detector
Figure 2.7.: TF-µSR experimental setup. Red lines represent external field flux lines. Black and orange arrows indicate particles’
spin and momentum direction, respectively.
Transverse-field configuration (TF-µSR) In this configuration the external field is applied perpendicularly to the initial muon spin di- rection (Fig. 2.7). The muon spin precesses about the composition of transverse and internal field (if any). The TF-µSR configuration can be used to measure the magnetic field distribution of the vortex lattice in a type-II superconductor or the µ Knight shift in metallic systems.
2.5. Probing magnetic order
Since in this thesis we deal with paramagnetic and magnetically order systems only, in the next section we focus on the description of the interactions which involve the muon spin in a magnetic sample.
2.5.1. Contributions to the local field at the muon site In the semi-classical description of the magnetic field at the muon site, the interaction between the material and the muon spin Sµis written as
H = ¯hγµSµ· Bµ, (2.16)
Sample geometry n factor Cylinder in parallel field 0 Cylinder in transverse field 1/2
Thin plate in perpendicular field 1
Table 2.1.: The demagnetizing factor n for various geometries.
where Bµ is the total field at the muon site.
The main contributions to the total field at the muon site Bµcome from the dipolar field, the hyperfine field and the demagnetizing field:
Bµ= Bdip+ Bhf+ Bdem+ µ0Happ , (2.17) where Bhf originates from unpaired electron spin polarization at the muon site and is commonly evaluated as a contact hyperfine field Bcontand/or a transferred hyperfine field Btrans. Finally, Happ is the externally applied field.
The crucial physical parameters governing the size of these contri- butions are the distance between the µ+ and the magnetic ions, the magnetic moments of the ordered magnetic phase, the density of spin polarised electrons at the µ+ site and the shape of the sample in the case of ferromagnets or ferrimagnets.
The dipolar field can be written, assuming a classical moment m centred at the atomic positions of magnetic atoms, as
Bdip(r) = µ0 4π
3ri(mi· ri) ri5 −mi
(2.18) where mi is the magnetic moment of atom i and ri is the distance between atom i and the muon site.
The local field at the muon sites are is usually evaluated in direct space by introducing the so-called Lorentz construction. The value B0µ is evaluated for all atoms within a sphere with radius rLfrom the muon site. The sphere is assumed to reside in a single magnetic domain and the magnetic moments outside the Lorentz sphere are regarded as a continuous and homogeneous magnetization density and contribute to an additional field BL. Within a single magnetic domain, BL= µ30Ms
2.5. Probing magnetic order with Ms being the saturation magnetization of the magnetic domain.
The dipolar field at the muon site is then Bµ= B0µ+BL. On standard desktop computers, summations of millions of atoms can be performed in a few seconds.
The demagnetizing field Bdem arises from the dipoles on the surface of the sample. For ellipsoidal samples Bdem = −µ0DMs where D is the demagnetization tensor and Ms is the magnetization of the sample. Of course, both Bdem and BL vanish in antiferromagnets.
In the case of ferro/ferrimagnets, for the special case of ellipsoids, the demagnetization field is linearly related to the magnetization by a geometry dependent constant called the demagnetizing factor n.
Its value is reported in Tab. 2.1 for various geometries. For non- ellipsoidal samples, Bdem is inhomogeneous and broadens the local field distribution at the muon site(s).
The contact hyperfine field or contact Fermi field can be written as
|Bcont(r0)| = −2
3µ0geµB(nup(r0) − ndn(r0)) (2.19) for a spherical electronic cloud surrounding the muon in position r0 .
Two additional contributions are worth citing: in metals with un- paired d or f electrons, a RKKY contribution can take place while in insulators a transferred hyperfine field, Btrans, can contribute to the local fields at the muon site. The former arises from a second order process which involves the polarisation of conduction electrons by the localised d or f shells having unpaired electrons and a subsequent local field at the muon site is produced by the contact hyperfine in- teraction. The latter stems from the overlap between the muon wave function and the localised magnetic wave functions.
Finally, a few symmetry considerations apply for the contributions to the local field appearing in Eq. 2.17. In a ferromagnet, Bcont lies in the same direction of the domain magnetization. By symmetry considerations Bdip vanishes for a muon site in a system of dipoles with cubic point group symmetry (m¯3m).
2.5.2. Static and dynamic local fields
We consider now the effect of a static local magnetic field B at the muon site forming an angle θ with the initial muon spin direction. In the semi-classical picture, the muon spin precess around the magnetic field forming a cone of half-angle θ between the spin and the local magnetic field direction. The muon polarization as a function of time, σ(t), projected in the direction of the initial spin polarization is
σ(t) = cos2θ + sin2θ cos(γµ|B| t) (2.20) Let f (B) be the magnetic field distribution function at the muon site, then the spin relaxation function G(t) is formally given by
G(t) = Z
f (B)hcos2θ + sin2θ cos(γµ|B| t)idB . (2.21) If the internal field distribution is only a function of |B|, as it is the case, for example, for an antiferromagnetic (AFM) polycrystalline sample, one has
G(t) = Z ∞
f (|B|)hcos2θ + sin2θ cos (γµ|B| t)i4πB2dB (2.22) By integrating over angular variables, G(t) can be written as
G(t) = 1 3 +2
f (|B|) cos (γµ|B| t) 4πB2dB (2.23) If the local magnetic field has a well defined modulus and randomly distributed directions, i.e.
f (|B|) = δ(B − ¯B) (2.24) substituting Eq. 2.24 and integrating gives
G(t) = 1 3 +2
3cos(γµBt)¯ (2.25) This is what would be observed in ideal powdered magnetic sam- ples. However, the delta distribution of Eq. 2.24 is never detected in real materials since the local magnetic field is usually broadened by
2.5. Probing magnetic order the presence of vacancies, self-interstitials, magnetic impurities, dis- locations or domain walls. A more realistic approach is to consider a Gaussian distribution for the internal magnetic fields in the i-th direction
f (Bi) = √γµ
2π∆exp −γµ2(Bi− ¯Bi)2 2∆2
(2.26) where i = x, y, z identify the three field components. Let the local field at the muon site be the sum of two components with angular independent distributions given by Eq. 2.24 and Eq. 2.26 and assume for the latter ¯Bi equal zero. The integration over angular variables gives the distribution 
f (|B|) = 1
(2π)3/2∆ ¯B|B|exp −B¯2+ B2 2∆2
(2.27) which is known as Koptev-Tarasov distribution. From Eq. 2.23, for B ∆, one has¯
G(t) = 1 3+2
3cos(γµBt) exp¯ −γµ2∆2t2 2
(2.28) which evidence a damping of the oscillating component which origi- nates from the de-phasing of the muon spins due to the presence of a distribution of local fields. This is the typical signal found in static magnetically ordered samples, characterised by disorder or impurities.
Considering the Gaussian distributions of Eq. 2.26 with ¯Bx,y,z = 0 for all the three directions, integration of Eq. 2.21 gives
G(t) = 1 3+2
3(1 − γµ2∆2t2) exp −γµ2∆2t2 2
. (2.29) Eq. 2.29 is known as static Kubo-Toyabe relaxation function (Fig. 2.8b) and describes the µSR signal of randomly oriented classical dipoles.
This is the case, for example, of nuclear magnetic dipoles but poten- tially also static magnetic disorder of electronic origin.
Finally, if a magnetic field is applied along the i-th direction par- allel to the muon spin (LF configuration), ¯Bi 6= 0 and the integral of Eq. 2.22 yields :
ρ(Bi) µ+ Local field
0 1 2 3 4 5 6
γµ∆ = 0.5 µs−1 γµ∆ = 1 µs−1 γµ∆ = 3 µs−1 γµ∆ = 6 µs−1
Figure 2.8.: In (a) a sketch depicting randomly oriented local moments in a lattice. The resulting distribution of fields projected onto an axis is showed on the left. In (b) the Kubo-Toyabe relaxation function for several values of ∆ is plotted.
G(t) = 1 −2∆2 B¯i2
1 − cos(γµBt) exp¯ −γµ2∆2t2 2
B¯3i) (2.30) If ¯Bi ∆, the polarisation of the muon is fixed and the spin will be aligned along the i-direction.
Up to now we have only considered static local fields on the timescales investigated (which depend on γµ). When dynamical fluctuations of internal field sets in, they introduce an additional relaxation processes which is independent from magnetic disorder.
There are two possible reasons why a magnetic system could ap- pear dynamic in µSR signals. Either fluctuations of the local field are
2.6. Quantum description of the dipolar interaction present or the muon is dynamic, i.e. it diffuses in a static spin sys- tem. A solution for a dynamical modulation of local magnetic field, resulting either from the muon hopping from site to site or from the internal fields instantly changing as a consequence phase shifts, can be accounted for within the strong collision Markovian approximation .
For slow hopping rate in a local moment environment described by a Gaussian field distribution, the asymptotic form of static Kubo- Toyabe distribution (Eq. 2.29) is modified and may be evaluated ap- proximately as
G(t) ∼ 1 3exp
(2.31) where the fluctuation frequency ν is the inverse of the hopping cor- relation time (τc = ν−1). Eq. 2.31 shows the signature of dynamic contributions to the asymmetry, i.e the loss of the 1/3 tail. Indeed in the case of slow dynamics the asymptote progressively reduces from1/3
to 0 as a function of ν. In the fast fluctuation limit, the depolarisation has the form
G(t) ∼ exp(−λt) . (2.32)
with λ = 2(γµ∆)2τc. This is the so called “motional narrowing limit”
in which the depolarisation of the asymmetry signal is inhibited by the fast hopping rate. In the intermediate fluctuation rate, G(t) is
G(t) = exp
ν2 (exp(−νt) − 1 + νt)
(2.33) This is the so called “Abragam relaxation function” [38, 39].
2.6. Quantum description of the dipolar interaction
All of the above results are based on a semi-classical description of the electromagnetic interaction taking place between the muon spin and the localised moments in a sample. Celio and Meier were the first to consider the dipolar interaction between the muon and the nuclei in a pure quantum-mechanical fashion in the context of µSR . They
0 2 4 6 8 10 Time [µs]
0.10.2 0.30.4 0.50.6 0.70.8 0.91.0
Figure 2.9.: The time evolution Gp(t) of the normalised asymmetry for an axial F-µ-F site with ωd = 0.16 MHz in a powdered sample.
showed that the difference between a Kubo-Toyabe function, which is expected from classical arguments, and a quantum description of the same interaction produces small differences that can be observed within the µSR time window. However, a marked departure from the classically expected trend was first observed in LiF . Indeed in fluorides, because of the high nuclear moment of F nuclei (19F has spin I = 1/2 and ∼ 100% natural abundance) and of the high electronegativity of this element, the interaction, commonly referred as F-µ-F†, is more pronounced. Here we briefly revise the analysis proposed in the article by Brewer and co-workers for LiF.
An entangled quantum state develops between the muon and the surrounding nuclei and the system may be described with the following Hamiltonian
4πr3 [Si· Sj − 3(Si· ˆr)(Sj· ˆr)] , (2.34) where r is the vector between spins Si and Sj of either the fluorine nuclei or the muon, which have gyromagnetic ratios γi and γj. The muon depolarisation is given by:
†We mention that “F-Mu-F” is probably a more appropriate label for this
“molecule-in-a-crystal”  structure. Indeed, Mu identifies both the µ+ particle and the electronic orbital forming the bonds with the F nuclei. However, we prefer to stick with the original and widely used notation.